Introduction to Materials & Testing

1 / 30

# Introduction to Materials & Testing - PowerPoint PPT Presentation

## Introduction to Materials & Testing

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -
##### Presentation Transcript

1. Introduction to Materials & Testing CON 251 Materials Testing

2. Types of Testing • Destructive testing is changes the dimensions or physical and structural integrity of the specimen. (It is essentially destroyed during the test) e.g., Tensile, Compression, Shear and Rockwell Hardness • Non-Destructive testing does not affect the structural integrity of the sample. ( A measurement that does not effect the specimen in any way) e.g., weighing, measurements etc.

3. Mechanical Testing UltimateTensile Strength - The maximum tensile stress that a material is capable of developing during a test. Load- Applied force either pounds or newtons Stress - The intensity of the internally-distributed forces or components of forces that resist a change in the form of a body. Commonly measured in units dealing with force per unit area, such as pounds per square inch (PSI or lb/in2) or Megapascals (Mpa). The three basic types of stress are tension, compression, and shear. The first two, tension and compression, are called direct stresses. Elastic Limit - The greatest amount of stress a material can develop without taking a permanent set. Percent Elongation - The total percent strain that a specimen develops during testing.

4. Principal properties determined through tensile testing include yield strength, tensile strength, ductility (based on the percent elongation and percent reduction in area), modulus of elasticity, and visual characteristics of the fracture. For brittle materials, which do not show a marked yield or ductility, data is collected for tensile strength and type and condition of fracture. Expected Results The results of tensile testing can be used to plot a stress-strain curve which illustrates the tensile properties of the material. Stress (in pounds per square inch or Pascal's) is plotted on the vertical axis while strain (inches per inch, millimeters per millimeter, or unit less) is plotted along the horizontal. As the load is applied, the curve is proportional and this period of linearity is termed the elastic region. Once the curve deviates from a straight line and begins to yield, the material has reached the proportional limit. Once the material has yielded, it exhibits plastic behavior or plasticity. Brittle materials do not exhibit much yield and are, therefore, less curved than ductile materials.

5. Modulus of Elasticity - Also known as Young’s modulus; calculated by finding the slope of the stress-strain curve for a given material within the range of its linear proportionality between stress and strain. Proportional Limit - The greatest stress a material can develop without deviating from linearity between stress and strain. Otherwise stated, the greatest stress developed in a material within its elastic range. Percent Reduction in Area - The difference between the original and final cross-sectional areas of a test piece, expressed as a percentage. Yield Point – Also referred to as Elastic Limit, is the point at which any additional stress will result in permanent deformation. Yield Strength - The stress at which a material exhibits a specified limiting permanent set.

6. Tensile Test - Introduction • The tensile test is a common test performed on metals, wood, plastics, and most other materials. • Tensile loads are those that tend to pull the specimen apart, putting the specimen in tension. They can be performed on any specimen of known cross-sectional area and gage length to which a uniform tensile load can be applied. • Tensile tests are used to determine the mechanical behavior of materials under static, axial tensile, or stretch loading. • ASTM standards for common tensile tests may be found in sections E8 (metals), D638 (plastics), D2343 (fibers), D897 (adhesives), D987 (paper), and D412 (rubber).

7. The engineering stress is: P is the load in lbs. on the specimen and A0 is the original cross-sectional area near the center of the specimen. On the other hand, the true stress is the load divided by the true area, which continues to be smaller by the tensile load. The true stress continues to increase to the point of fracture, while the engineering stress decreases to the point of fracture due to the increasing load and the constant cross-sectional area.

8. The engineering strain is: l is the gage length at a given load and l0is the original gage length with zero load

9. Modulus of Elasticity • The slope of the stress-strain curve in the elastic deformation region is the modulus of elasticity, which is known as Young's modulus

10. Material Fracture: Background Stress-Strain CurveThis stress-strain curve is produced from the tensile test.

11. Stress Strain for Different Materials

12. Tensile Testing - Procedure • Tensile tests are used to determine the tensile properties of a material, including the tensile strength. The tensile strength of a material is the maximum tensile stress that can be developed in the material. • In order to conduct a tensile test, the proper specimen must be obtained. This specimen should conform to ASTM standards for size and features. Prior to the test, the cross-sectional area may be calculated and a pre-determined gage length marked. • The specimen is then loaded into a machine set up for tensile loads and placed in the proper grippers. Once loaded, the machine can then be used to apply a steady, continuous tensile load. • Data is collected at pre-determined points or increments during the test. Depending on the material and specimen being tested, data points may be more or less frequent. Data include the applied load and change in gage length. The load is generally read from the machine panel in pounds or kilograms.

13. The change in gage length is determined using an extensometer. An extensometer is firmly fixed to the machine or specimen and relates the amount of deformation or deflection over the gage length during a test. • While paying close attention to the readings, data points are collected until the material starts to yield significantly. This can be seen when deformation continues without having to increase the applied load. Once this begins, the extensometer is removed and loading continued until failure. Ultimate tensile strength and rupture strength can be calculated from this latter loading. • Once data have been collected, the tensile stress developed and the resultant strain can be calculated. Stress is calculated based on the applied load and cross-sectional area. Strain is the change in length divided by the original length.

14. Compression Testing - Introduction • Simplistically, compression testing is the opposite of tensile testing. A compressive load tends to squeeze or compact the specimen. The choice of a compression test over other types of testing largely depends on the type of loading the material will see during application or service. • Metals and many plastics, for example, are more efficient at resisting tensile loads. Therefore, they are more commonly tested using tensile loading, depending on the application, of course. Materials, such as concrete, brick, and some ceramic products, are more often used in applications for their compressive loading properties and are, therefore, tested in compression. Again, it is important to choose the test that best reflects the loads and conditions the material will be subjected to in application or service.

15. Compression Testing – Procedure During a typical compression test, data are collected regarding the applied load, resultant deformation or deflection, and condition of the specimen. For brittle materials, the compressive strength is relatively easy to obtain, showing marked failure. However, for ductile materials, the compressive strength is generally based on an arbitrary deformation value. Ductile materials do not exhibit the sudden fractures that brittle materials present. They tend to buckle and "barrel out".

16. Barreling or Bulging of a Sample under Compressive Loads

17. Prior to this and any test, the dimensions of the specimen should be measured with adequate precision using proper instruments. Once these measurements have been taken and recorded, the specimen should be loaded into the testing machine. • In compression testing, and testing in general, care should be taken to insure that the axis of the specimen is centered and aligned with the axis of loading. • Loading rates should be steady and continuous. Rates vary, but a general figure is 0.005 inches per minute strain rate. Loading rates typically range from 500-1000 lb/min.

18. As in most tests of mechanical properties, the loading rate can adversely affect the results if you get carried away. Loading continues at this rate up to approximately one-half of the anticipated strength and, then, should be reduced to allow for more frequent data collection. In this way, subtle changes can be observed in the specimen's behavior. • As in all of these tests, please observe proper safety procedures. Obtain and properly wear personal protective equipment. Some of these materials exhibit violent fractures with explosive results.